#------------------------------------------------------------------------------
#$Date: 2016-03-23 03:56:46 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179270 $
#$URL: svn://www.crystallography.net/cod/cif/4/31/90/4319070.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4319070
loop_
_publ_author_name
'Charlotte du Peloux'
'Anne Dolbecq'
'Pierre Mialane'
'Jérôme Marrot'
'Eric Rivière'
'Francis Sécheresse'
_publ_contact_author
;
        Pr. F. Secheresse
        Institut Lavoisier, IREM, UMR CNRS C 8637
        Université de Versailles Saint-Quentin-en-Yvelines
        45 Avenue des Etats Unis
        78035 Versailles cedex
        France
;
_publ_contact_author_email       Secheres@chimie.uvsq.fr
_publ_contact_author_fax         '(33) 1 39 25 43 81'
_publ_contact_author_phone       '(33) 1 39 25 43 83'
_publ_section_title
;
 A New Two-Dimensional Molybdenum(V) Nickel Phosphate Built Up of
 [H18(Mo16O32)Ni16(PO4)26(OH)6(H2O)8]18- Wheels
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              7100
_journal_page_last               7104
_journal_paper_doi               10.1021/ic0204880
_journal_volume                  41
_journal_year                    2002
_chemical_formula_sum            'H172 Mo16 Na6 Ni22 O216 P26'
_chemical_formula_weight         7399.20
_chemical_name_systematic
;
   ?
;
_space_group_IT_number           66
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2 2c'
_symmetry_space_group_name_H-M   'C c c m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   23.999(4)
_cell_length_b                   36.595(6)
_cell_length_c                   20.445(4)
_cell_measurement_reflns_used    24528
_cell_measurement_temperature    296(2)
_cell_volume                     17956(5)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SHELXTL'
_computing_molecular_graphics    'Diamond Brandenburg'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.933
_diffrn_measured_fraction_theta_max 0.933
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1140
_diffrn_reflns_av_sigmaI/netI    0.0998
_diffrn_reflns_limit_h_max       31
_diffrn_reflns_limit_h_min       -31
_diffrn_reflns_limit_k_max       29
_diffrn_reflns_limit_k_min       -50
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_limit_l_min       -27
_diffrn_reflns_number            61917
_diffrn_reflns_theta_full        30.01
_diffrn_reflns_theta_max         30.01
_diffrn_reflns_theta_min         1.01
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    3.721
_exptl_absorpt_correction_T_max  0.9293
_exptl_absorpt_correction_T_min  0.5874
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick, 1996)'
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    2.737
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       parallelepiped
_exptl_crystal_F_000             14576
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.02
_refine_diff_density_max         3.447
_refine_diff_density_min         -1.343
_refine_diff_density_rms         0.332
_refine_ls_extinction_coef       0.000086(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.097
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     741
_refine_ls_number_reflns         12560
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.097
_refine_ls_R_factor_all          0.1447
_refine_ls_R_factor_gt           0.0753
_refine_ls_shift/su_max          0.013
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0730P)²+531.1516P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1619
_refine_ls_wR_factor_ref         0.1993
_reflns_number_gt                7601
_reflns_number_total             12560
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic0204880.cif
_cod_data_source_block           cap5
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to the built-in table from CIF Core
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 
;
_cod_database_code               4319070
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z+1/2'
'x, -y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z'
'x, -y, z-1/2'
'-x, y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
'-x+1/2, y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.137422(14) 0.144299(10) 0.158251(17) 0.02009(8) Uani 1 1 d . . .
Mo2 Mo 0.013937(14) 0.357217(9) 0.106748(17) 0.01793(8) Uani 1 1 d . . .
Mo3 Mo 0.094037(14) 0.319647(9) 0.158796(17) 0.01977(8) Uani 1 1 d . . .
Mo4 Mo 0.084127(14) 0.090154(10) 0.104938(19) 0.02276(9) Uani 1 1 d . . .
Ni1 Ni 0.23241(2) 0.081004(14) 0.06875(3) 0.02079(13) Uani 1 1 d . . .
Ni2 Ni -0.01635(2) 0.261266(14) 0.07813(3) 0.02080(13) Uani 1 1 d . . .
Ni3 Ni 0.35394(2) 0.097063(14) 0.06913(2) 0.01871(12) Uani 1 1 d . . .
Ni4 Ni 0.00401(2) 0.175403(15) 0.07971(3) 0.02562(14) Uani 1 1 d . . .
Ni5 Ni 0.5000 0.0000 0.07695(4) 0.0288(2) Uani 1 2 d S . .
Ni6 Ni 0.13603(5) -0.05535(4) -0.05504(7) 0.0199(3) Uani 0.38 1 d P . .
Ni7 Ni 0.2500 0.2500 0.0000 0.0261(3) Uani 1 4 d S . .
Ni8 Ni 0.28949(7) 0.16986(4) 0.44637(10) 0.0386(5) Uani 0.38 1 d P . .
P1 P -0.08090(6) 0.32593(4) 0.0000 0.0204(4) Uani 1 2 d S . .
P2 P 0.11306(6) 0.33012(4) 0.0000 0.0182(4) Uani 1 2 d S . .
P3 P 0.47253(6) 0.07442(4) 0.0000 0.0171(3) Uani 1 2 d S . .
P4 P 0.16107(7) 0.14023(4) 0.0000 0.0244(4) Uani 1 2 d S . .
P5 P 0.22221(4) 0.35786(3) 0.17565(5) 0.0221(3) Uani 1 1 d . . .
P6 P 0.13650(7) 0.02982(4) 0.0000 0.0248(4) Uani 1 2 d S . .
P7 P 0.07827(4) 0.22836(3) 0.17888(5) 0.0205(3) Uani 1 1 d . . .
P8 P -0.09836(6) 0.20968(4) 0.0000 0.0244(4) Uani 1 2 d S . .
P9 P -0.02297(6) 0.09696(4) 0.0000 0.0279(4) Uani 1 2 d S . .
P10 P 0.30624(6) 0.03474(4) 0.16321(6) 0.0344(3) Uani 1 1 d . . .
O1 O 0.16331(11) 0.09772(8) 0.11940(13) 0.0225(7) Uani 1 1 d . . .
O2 O 0.06300(11) 0.14079(8) 0.11962(14) 0.0246(8) Uani 1 1 d . . .
O3 O 0.22003(12) 0.15957(8) 0.17356(15) 0.0271(8) Uani 1 1 d . . .
O4 O 0.12325(12) 0.19900(8) 0.17483(15) 0.0281(8) Uani 1 1 d . . .
O5 O 0.15713(12) 0.16532(7) 0.06064(14) 0.0224(7) Uani 1 1 d . . .
O6 O -0.06040(12) 0.34606(8) 0.06187(14) 0.0231(7) Uani 1 1 d . . .
O7 O 0.00485(12) 0.40726(7) 0.06191(14) 0.0225(7) Uani 1 1 d . . .
O8 O 0.05142(16) 0.34334(10) 0.0000 0.0190(10) Uani 1 2 d S . .
O9 O -0.01623(12) 0.37223(8) 0.17567(14) 0.0246(8) Uani 1 1 d . . .
O10 O 0.09192(11) 0.36967(7) 0.12175(13) 0.0204(7) Uani 1 1 d . . .
O11 O 0.11038(13) 0.26443(8) 0.16975(16) 0.0308(9) Uani 1 1 d . . .
O12 O 0.02298(11) 0.30508(7) 0.11899(13) 0.0201(7) Uani 1 1 d . . .
O13 O 0.06412(14) 0.06961(9) 0.17552(16) 0.0360(9) Uani 1 1 d . . .
O14 O 0.00848(12) 0.08335(8) 0.06141(17) 0.0330(9) Uani 1 1 d . . .
O15 O 0.10422(12) 0.04176(8) 0.06207(16) 0.0307(9) Uani 1 1 d . . .
O16 O 0.25167(14) 0.03810(9) 0.12531(18) 0.0410(10) Uani 1 1 d . . .
O17 O 0.17960(12) 0.32653(8) 0.17384(16) 0.0302(8) Uani 1 1 d . . .
O18 O 0.12391(12) 0.30620(7) 0.06008(14) 0.0234(7) Uani 1 1 d . . .
O19 O 0.07811(13) 0.32590(9) 0.23827(15) 0.0325(9) Uani 1 1 d . . .
O20 O 0.10956(17) 0.11285(12) 0.0000 0.0263(11) Uani 1 2 d S . .
O21 O 0.28568(11) 0.11505(8) 0.11954(13) 0.0221(7) Uani 1 1 d . . .
O22 O 0.03824(17) 0.25454(11) 0.0000 0.0234(11) Uani 1 2 d S . .
O23 O 0.19354(17) 0.04770(12) 0.0000 0.0273(12) Uani 1 2 d S . .
O24 O 0.29845(15) 0.07180(11) 0.0000 0.0204(10) Uani 1 2 d S . .
O25 O -0.05576(17) 0.28698(11) 0.0000 0.0224(11) Uani 1 2 d S . .
O26 O -0.05985(12) 0.21355(8) 0.05991(15) 0.0270(8) Uani 1 1 d . . .
O27 O -0.07753(13) 0.27133(9) 0.14926(15) 0.0335(9) Uani 1 1 d . . .
O28 O 0.03218(12) 0.22310(8) 0.12849(15) 0.0271(8) Uani 1 1 d . . .
O29 O 0.40915(16) 0.07540(10) 0.0000 0.0196(10) Uani 1 2 d S . .
O30 O 0.34723(17) 0.13670(11) 0.0000 0.0224(11) Uani 1 2 d S . .
O31 O 0.35671(13) 0.05157(8) 0.12636(15) 0.0297(8) Uani 1 1 d . . .
O32 O 0.05044(17) 0.18978(11) 0.0000 0.0272(11) Uani 1 2 d S . .
O33 O -0.04958(15) 0.15716(11) 0.15110(18) 0.0561(12) Uani 1 1 d . . .
O34 O 0.4977(2) 0.03852(10) 0.15087(17) 0.0536(12) Uani 1 1 d . . .
O35 O 0.49581(16) 0.03522(10) 0.0000 0.0199(10) Uani 1 2 d S . .
O36 O 0.58590(14) 0.00418(10) 0.07250(19) 0.0473(11) Uani 1 1 d . . .
O37 O -0.14347(17) 0.32478(12) 0.0000 0.0307(12) Uani 1 2 d S . .
O38 O -0.0255(2) 0.13932(13) 0.0000 0.0403(15) Uani 1 2 d S . .
O39 O 0.21526(15) 0.37892(10) 0.24179(15) 0.0420(10) Uani 1 1 d . . .
O40 O 0.14073(19) -0.01184(11) 0.0000 0.0369(14) Uani 1 2 d S . .
O41 O 0.05244(13) 0.22675(9) 0.24857(15) 0.0349(9) Uani 1 1 d . . .
O42 O -0.14890(17) 0.23410(11) 0.0000 0.0343(13) Uani 1 2 d S . .
O43 O -0.12276(18) 0.16910(12) 0.0000 0.0378(14) Uani 1 2 d S . .
O44 O -0.08054(19) 0.08104(13) 0.0000 0.0449(16) Uani 1 2 d S . .
O45 O 0.29891(19) 0.05066(12) 0.23225(18) 0.0635(14) Uani 1 1 d . . .
O46 O 0.32038(16) -0.00735(10) 0.17080(19) 0.0550(12) Uani 1 1 d . . .
O47 O 0.1693(3) 0.23933(17) 0.0286(4) 0.050(2) Uani 0.50 1 d P . .
O48 O 0.3244(2) 0.22250(10) 0.41397(18) 0.0557(13) Uani 1 1 d . . .
O49 O 0.3349(3) 0.1561(3) 0.3587(4) 0.081(3) Uani 0.50 1 d P . .
O50 O 0.2137(4) -0.1542(3) -0.1077(7) 0.113(5) Uani 0.50 1 d P . .
O51 O 0.21787(16) 0.11968(11) 0.0000 0.0252(11) Uani 1 2 d S . .
O52 O 0.12606(13) 0.13150(9) 0.23593(16) 0.0351(9) Uani 1 1 d . . .
O53 O 0.2022(2) -0.07781(16) 0.0000 0.060(2) Uani 1 2 d S . .
O54 O 0.0691(3) -0.02987(17) -0.0997(4) 0.0464(19) Uani 0.50 1 d P . .
O55 O 0.2709(4) 0.1173(3) 0.5000 0.041(2) Uiso 0.50 2 d SP . .
O56 O 0.1883(3) -0.0288(2) -0.1222(5) 0.103(3) Uani 0.50 1 d P . .
O57 O 0.1375(4) -0.1017(3) -0.1190(5) 0.072(3) Uiso 0.50 1 d P . .
O58 O 0.2252(4) -0.0222(3) -0.0718(5) 0.084(3) Uiso 0.50 1 d P . .
O59 O 0.2450(5) 0.1951(3) 0.5000 0.053(3) Uiso 0.50 2 d SP . .
O60 O 0.2590(3) 0.2088(2) 0.0669(4) 0.0484(19) Uiso 0.50 1 d P . .
O1W O 0.0000 0.11928(15) 0.2500 0.0527(17) Uani 1 2 d S . .
O2W O -0.0821(3) 0.42075(19) 0.2510(3) 0.047(2) Uani 0.50 1 d P . .
O3W O 0.1772(3) 0.0518(2) 0.2481(4) 0.143(3) Uani 1 1 d . . .
O4W O 0.4319(5) 0.0000 0.2500 0.186(7) Uani 1 2 d S . .
O5W O 0.2218(4) 0.2435(3) 0.2132(6) 0.106(5) Uani 0.50 1 d P . .
O6W O 0.1568(7) -0.1991(3) -0.1761(5) 0.144(5) Uani 0.50 1 d P . .
O7W O 0.6211(7) 0.0807(4) 0.1043(8) 0.049(4) Uiso 0.25 1 d P . .
O8W O -0.1229(7) 0.4217(5) 0.0492(9) 0.063(5) Uiso 0.25 1 d P . .
O9W O 0.1985(7) -0.1246(5) -0.0780(9) 0.060(5) Uiso 0.25 1 d P . .
O10W O 0.0631(10) -0.0046(9) -0.2316(13) 0.125(9) Uiso 0.25 1 d P . .
Na1 Na 0.2042(3) 0.2336(3) 0.1610(4) 0.059(3) Uani 0.25 1 d P . .
Na2 Na -0.1037(6) 0.4500(5) 0.1624(7) 0.136(6) Uani 0.25 1 d P . .
Na3 Na 0.2906(4) -0.0123(2) 0.0000 0.082(3) Uani 0.50 2 d SP . .
Na4 Na 0.0000 0.0000 -0.024(2) 0.19(2) Uani 0.25 2 d SP . .
Na5 Na 0.2769(9) 0.2564(7) 0.3390(8) 0.280(9) Uani 0.25 1 d P . .
Na6 Na -0.2148(17) 0.4238(11) 0.064(2) 0.147(13) Uiso 0.13 1 d P . .
Na7 Na 0.2582(12) -0.0704(7) -0.1248(13) 0.091(8) Uiso 0.13 1 d P . .
Na8 Na 0.2013(10) -0.1082(7) -0.1867(12) 0.076(6) Uiso 0.13 1 d P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O52 Mo1 O2 102.44(14) . . ?
O52 Mo1 O1 100.97(14) . . ?
O2 Mo1 O1 93.90(12) . . ?
O52 Mo1 O4 95.10(14) . . ?
O2 Mo1 O4 88.82(12) . . ?
O1 Mo1 O4 162.70(12) . . ?
O52 Mo1 O3 95.01(14) . . ?
O2 Mo1 O3 161.20(12) . . ?
O1 Mo1 O3 89.58(11) . . ?
O4 Mo1 O3 82.62(12) . . ?
O52 Mo1 O5 174.47(14) . . ?
O2 Mo1 O5 81.52(11) . . ?
O1 Mo1 O5 82.48(11) . . ?
O4 Mo1 O5 81.04(11) . . ?
O3 Mo1 O5 80.63(11) . . ?
O52 Mo1 Mo4 95.98(12) . . ?
O2 Mo1 Mo4 48.04(8) . . ?
O1 Mo1 Mo4 47.92(8) . . ?
O4 Mo1 Mo4 136.84(8) . . ?
O3 Mo1 Mo4 137.40(8) . . ?
O5 Mo1 Mo4 89.54(7) . . ?
O52 Mo1 Na1 107.91(18) . . ?
O2 Mo1 Na1 117.84(16) . . ?
O1 Mo1 Na1 129.85(16) . . ?
O4 Mo1 Na1 36.61(16) . . ?
O3 Mo1 Na1 48.53(16) . . ?
O5 Mo1 Na1 66.66(15) . . ?
Mo4 Mo1 Na1 155.22(14) . . ?
O9 Mo2 O12 105.22(13) . . ?
O9 Mo2 O10 101.87(13) . . ?
O12 Mo2 O10 95.88(11) . . ?
O9 Mo2 O6 93.77(13) . . ?
O12 Mo2 O6 87.65(11) . . ?
O10 Mo2 O6 162.40(11) . . ?
O9 Mo2 O7 92.12(12) . . ?
O12 Mo2 O7 161.00(11) . . ?
O10 Mo2 O7 87.93(11) . . ?
O6 Mo2 O7 83.43(11) . . ?
O9 Mo2 O8 171.63(13) . . ?
O12 Mo2 O8 82.41(12) . . ?
O10 Mo2 O8 80.43(12) . . ?
O6 Mo2 O8 82.97(12) . . ?
O7 Mo2 O8 79.87(11) . . ?
O9 Mo2 Mo3 98.57(10) . . ?
O12 Mo2 Mo3 48.79(8) . . ?
O10 Mo2 Mo3 49.29(8) . . ?
O6 Mo2 Mo3 136.43(8) . . ?
O7 Mo2 Mo3 137.14(8) . . ?
O8 Mo2 Mo3 89.04(8) . . ?
O19 Mo3 O12 103.86(13) . . ?
O19 Mo3 O10 103.72(14) . . ?
O12 Mo3 O10 94.02(11) . . ?
O19 Mo3 O11 94.09(14) . . ?
O12 Mo3 O11 86.81(12) . . ?
O10 Mo3 O11 161.39(12) . . ?
O19 Mo3 O17 93.70(14) . . ?
O12 Mo3 O17 161.16(12) . . ?
O10 Mo3 O17 88.29(11) . . ?
O11 Mo3 O17 85.16(12) . . ?
O19 Mo3 O18 171.94(13) . . ?
O12 Mo3 O18 80.90(11) . . ?
O10 Mo3 O18 82.20(11) . . ?
O11 Mo3 O18 79.57(11) . . ?
O17 Mo3 O18 80.90(12) . . ?
O19 Mo3 Mo2 98.95(11) . . ?
O12 Mo3 Mo2 47.90(8) . . ?
O10 Mo3 Mo2 48.25(8) . . ?
O11 Mo3 Mo2 134.63(9) . . ?
O17 Mo3 Mo2 136.44(8) . . ?
O18 Mo3 Mo2 89.07(7) . . ?
O13 Mo4 O1 102.16(14) . . ?
O13 Mo4 O2 102.55(14) . . ?
O1 Mo4 O2 95.49(12) . . ?
O13 Mo4 O15 92.73(14) . . ?
O1 Mo4 O15 87.58(12) . . ?
O2 Mo4 O15 163.36(13) . . ?
O13 Mo4 O14 93.74(15) . . ?
O1 Mo4 O14 162.84(12) . . ?
O2 Mo4 O14 87.22(12) . . ?
O15 Mo4 O14 85.22(12) . . ?
O13 Mo4 O20 173.68(15) . . ?
O1 Mo4 O20 80.60(12) . . ?
O2 Mo4 O20 82.73(13) . . ?
O15 Mo4 O20 81.64(14) . . ?
O14 Mo4 O20 82.96(13) . . ?
O13 Mo4 Mo1 96.92(11) . . ?
O1 Mo4 Mo1 49.15(8) . . ?
O2 Mo4 Mo1 48.45(8) . . ?
O15 Mo4 Mo1 136.73(8) . . ?
O14 Mo4 Mo1 135.66(9) . . ?
O20 Mo4 Mo1 89.18(9) . . ?
O16 Ni1 O51 171.07(13) . . ?
O16 Ni1 O1 97.41(13) . . ?
O51 Ni1 O1 90.15(12) . . ?
O16 Ni1 O21 92.28(13) . . ?
O51 Ni1 O21 91.95(13) . . ?
O1 Ni1 O21 93.83(11) . . ?
O16 Ni1 O23 91.97(14) . . ?
O51 Ni1 O23 82.14(13) . . ?
O1 Ni1 O23 98.83(13) . . ?
O21 Ni1 O23 166.02(12) . . ?
O16 Ni1 O24 94.86(14) . . ?
O51 Ni1 O24 77.42(13) . . ?
O1 Ni1 O24 167.49(12) . . ?
O21 Ni1 O24 88.10(12) . . ?
O23 Ni1 O24 78.27(13) . . ?
O16 Ni1 Ni1 125.24(10) . 10 ?
O51 Ni1 Ni1 46.05(8) . 10 ?
O1 Ni1 Ni1 120.36(8) . 10 ?
O21 Ni1 Ni1 120.19(8) . 10 ?
O23 Ni1 Ni1 47.51(8) . 10 ?
O24 Ni1 Ni1 49.06(7) . 10 ?
O16 Ni1 Ni3 85.82(10) . . ?
O51 Ni1 Ni3 91.87(11) . . ?
O1 Ni1 Ni3 137.16(8) . . ?
O21 Ni1 Ni3 43.33(8) . . ?
O23 Ni1 Ni3 123.84(10) . . ?
O24 Ni1 Ni3 46.24(8) . . ?
Ni1 Ni1 Ni3 90.152(14) 10 . ?
O12 Ni2 O26 166.20(12) . . ?
O12 Ni2 O22 96.66(13) . . ?
O26 Ni2 O22 94.57(14) . . ?
O12 Ni2 O25 99.74(13) . . ?
O26 Ni2 O25 90.80(14) . . ?
O22 Ni2 O25 75.54(13) . . ?
O12 Ni2 O28 93.77(11) . . ?
O26 Ni2 O28 78.81(12) . . ?
O22 Ni2 O28 87.04(13) . . ?
O25 Ni2 O28 159.00(12) . . ?
O12 Ni2 O27 84.38(12) . . ?
O26 Ni2 O27 85.40(12) . . ?
O22 Ni2 O27 173.27(13) . . ?
O25 Ni2 O27 97.73(13) . . ?
O28 Ni2 O27 99.54(12) . . ?
O30 Ni3 O31 170.48(12) . . ?
O30 Ni3 O21 93.28(13) . . ?
O31 Ni3 O21 89.98(12) . . ?
O30 Ni3 O10 89.51(12) . 6 ?
O31 Ni3 O10 99.26(12) . 6 ?
O21 Ni3 O10 92.95(11) . 6 ?
O30 Ni3 O29 81.42(13) . . ?
O31 Ni3 O29 93.31(12) . . ?
O21 Ni3 O29 165.83(12) . . ?
O10 Ni3 O29 100.10(12) 6 . ?
O30 Ni3 O24 78.50(13) . . ?
O31 Ni3 O24 92.66(12) . . ?
O21 Ni3 O24 88.48(12) . . ?
O10 Ni3 O24 167.99(11) 6 . ?
O29 Ni3 O24 77.60(12) . . ?
O30 Ni3 Ni3 45.92(8) . 10 ?
O31 Ni3 Ni3 125.08(9) . 10 ?
O21 Ni3 Ni3 120.28(8) . 10 ?
O10 Ni3 Ni3 121.14(7) 6 10 ?
O29 Ni3 Ni3 47.53(7) . 10 ?
O24 Ni3 Ni3 48.92(7) . 10 ?
O30 Ni3 Ni1 93.52(11) . . ?
O31 Ni3 Ni1 82.65(9) . . ?
O21 Ni3 Ni1 43.89(8) . . ?
O10 Ni3 Ni1 136.83(8) 6 . ?
O29 Ni3 Ni1 122.95(10) . . ?
O24 Ni3 Ni1 46.08(8) . . ?
Ni3 Ni3 Ni1 89.848(14) 10 . ?
O32 Ni4 O33 172.18(15) . . ?
O32 Ni4 O2 95.70(14) . . ?
O33 Ni4 O2 87.08(13) . . ?
O32 Ni4 O26 94.16(14) . . ?
O33 Ni4 O26 84.08(14) . . ?
O2 Ni4 O26 167.79(12) . . ?
O32 Ni4 O28 89.39(13) . . ?
O33 Ni4 O28 97.62(14) . . ?
O2 Ni4 O28 95.76(11) . . ?
O26 Ni4 O28 77.14(11) . . ?
O32 Ni4 O38 74.99(14) . . ?
O33 Ni4 O38 97.40(15) . . ?
O2 Ni4 O38 98.29(14) . . ?
O26 Ni4 O38 91.21(15) . . ?
O28 Ni4 O38 159.89(13) . . ?
O35 Ni5 O35 78.82(17) . 9_655 ?
O35 Ni5 O34 97.58(13) . . ?
O35 Ni5 O34 176.09(14) 9_655 . ?
O35 Ni5 O34 176.09(14) . 2_655 ?
O35 Ni5 O34 97.58(13) 9_655 2_655 ?
O34 Ni5 O34 86.1(2) . 2_655 ?
O35 Ni5 O36 88.19(15) . . ?
O35 Ni5 O36 87.91(15) 9_655 . ?
O34 Ni5 O36 90.46(17) . . ?
O34 Ni5 O36 93.23(17) 2_655 . ?
O35 Ni5 O36 87.91(15) . 2_655 ?
O35 Ni5 O36 88.19(15) 9_655 2_655 ?
O34 Ni5 O36 93.23(17) . 2_655 ?
O34 Ni5 O36 90.46(17) 2_655 2_655 ?
O36 Ni5 O36 175.0(2) . 2_655 ?
O35 Ni5 Na2 95.1(3) . 6 ?
O35 Ni5 Na2 132.2(3) 9_655 6 ?
O34 Ni5 Na2 46.1(3) . 6 ?
O34 Ni5 Na2 88.5(3) 2_655 6 ?
O36 Ni5 Na2 44.3(3) . 6 ?
O36 Ni5 Na2 139.3(3) 2_655 6 ?
O35 Ni5 Na2 132.2(3) . 5_545 ?
O35 Ni5 Na2 95.1(3) 9_655 5_545 ?
O34 Ni5 Na2 88.5(3) . 5_545 ?
O34 Ni5 Na2 46.1(3) 2_655 5_545 ?
O36 Ni5 Na2 139.3(3) . 5_545 ?
O36 Ni5 Na2 44.3(3) 2_655 5_545 ?
Na2 Ni5 Na2 121.0(5) 6 5_545 ?
O40 Ni6 O44 95.65(16) . 9 ?
O40 Ni6 O54 86.1(2) . . ?
O44 Ni6 O54 86.7(2) 9 . ?
O40 Ni6 O53 88.10(19) . . ?
O44 Ni6 O53 91.05(18) 9 . ?
O54 Ni6 O53 173.5(2) . . ?
O40 Ni6 O56 88.0(3) . . ?
O44 Ni6 O56 173.4(3) 9 . ?
O54 Ni6 O56 88.1(3) . . ?
O53 Ni6 O56 94.5(3) . . ?
O40 Ni6 O57 175.1(3) . . ?
O44 Ni6 O57 89.0(3) 9 . ?
O54 Ni6 O57 95.8(3) . . ?
O53 Ni6 O57 90.3(3) . . ?
O56 Ni6 O57 87.6(4) . . ?
O40 Ni6 Ni6 54.82(8) . 10 ?
O44 Ni6 Ni6 55.38(9) 9 10 ?
O54 Ni6 Ni6 116.2(2) . 10 ?
O53 Ni6 Ni6 57.83(9) . 10 ?
O56 Ni6 Ni6 130.9(2) . 10 ?
O57 Ni6 Ni6 127.6(3) . 10 ?
O40 Ni6 Na7 109.5(5) . . ?
O44 Ni6 Na7 139.6(5) 9 . ?
O54 Ni6 Na7 125.0(5) . . ?
O53 Ni6 Na7 59.9(5) . . ?
O56 Ni6 Na7 42.7(5) . . ?
O57 Ni6 Na7 65.8(5) . . ?
Ni6 Ni6 Na7 115.6(5) 10 . ?
O60 Ni7 O60 83.8(4) 13 6 ?
O60 Ni7 O60 180.0(4) 13 . ?
O60 Ni7 O60 96.2(4) 6 . ?
O60 Ni7 O60 96.2(4) 13 10 ?
O60 Ni7 O60 180.0(3) 6 10 ?
O60 Ni7 O60 83.8(4) . 10 ?
O60 Ni7 O47 98.6(3) 13 6 ?
O60 Ni7 O47 76.7(3) 6 6 ?
O60 Ni7 O47 81.4(3) . 6 ?
O60 Ni7 O47 103.3(3) 10 6 ?
O60 Ni7 O47 76.7(3) 13 13 ?
O60 Ni7 O47 98.6(3) 6 13 ?
O60 Ni7 O47 103.3(3) . 13 ?
O60 Ni7 O47 81.4(3) 10 13 ?
O47 Ni7 O47 33.0(4) 6 13 ?
O60 Ni7 O47 81.4(3) 13 10 ?
O60 Ni7 O47 103.3(3) 6 10 ?
O60 Ni7 O47 98.6(3) . 10 ?
O60 Ni7 O47 76.7(3) 10 10 ?
O47 Ni7 O47 180.0(5) 6 10 ?
O47 Ni7 O47 147.0(4) 13 10 ?
O60 Ni7 O47 103.3(3) 13 . ?
O60 Ni7 O47 81.4(3) 6 . ?
O60 Ni7 O47 76.7(3) . . ?
O60 Ni7 O47 98.6(3) 10 . ?
O47 Ni7 O47 147.0(4) 6 . ?
O47 Ni7 O47 180.0(3) 13 . ?
O47 Ni7 O47 33.0(4) 10 . ?
O60 Ni7 Na1 122.1(3) 13 6 ?
O60 Ni7 Na1 44.2(3) 6 6 ?
O60 Ni7 Na1 57.9(3) . 6 ?
O60 Ni7 Na1 135.8(3) 10 6 ?
O47 Ni7 Na1 53.8(2) 6 6 ?
O47 Ni7 Na1 86.6(2) 13 6 ?
O47 Ni7 Na1 126.2(2) 10 6 ?
O47 Ni7 Na1 93.4(2) . 6 ?
O60 Ni7 Na1 57.9(3) 13 10 ?
O60 Ni7 Na1 135.8(3) 6 10 ?
O60 Ni7 Na1 122.1(3) . 10 ?
O60 Ni7 Na1 44.2(3) 10 10 ?
O47 Ni7 Na1 126.2(2) 6 10 ?
O47 Ni7 Na1 93.4(2) 13 10 ?
O47 Ni7 Na1 53.8(2) 10 10 ?
O47 Ni7 Na1 86.6(2) . 10 ?
Na1 Ni7 Na1 180.0 6 10 ?
O60 Ni7 Na1 44.2(3) 13 13 ?
O60 Ni7 Na1 122.1(3) 6 13 ?
O60 Ni7 Na1 135.8(3) . 13 ?
O60 Ni7 Na1 57.9(3) 10 13 ?
O47 Ni7 Na1 86.6(2) 6 13 ?
O47 Ni7 Na1 53.8(2) 13 13 ?
O47 Ni7 Na1 93.4(2) 10 13 ?
O47 Ni7 Na1 126.2(2) . 13 ?
Na1 Ni7 Na1 138.4(3) 6 13 ?
Na1 Ni7 Na1 41.6(3) 10 13 ?
O60 Ni7 Na1 135.8(3) 13 . ?
O60 Ni7 Na1 57.9(3) 6 . ?
O60 Ni7 Na1 44.2(3) . . ?
O60 Ni7 Na1 122.1(3) 10 . ?
O47 Ni7 Na1 93.4(2) 6 . ?
O47 Ni7 Na1 126.2(2) 13 . ?
O47 Ni7 Na1 86.6(2) 10 . ?
O47 Ni7 Na1 53.8(2) . . ?
Na1 Ni7 Na1 41.6(3) 6 . ?
Na1 Ni7 Na1 138.4(3) 10 . ?
Na1 Ni7 Na1 180.0(3) 13 . ?
O59 Ni8 O37 95.5(3) . 15_556 ?
O59 Ni8 O49 158.7(4) . . ?
O37 Ni8 O49 94.2(2) 15_556 . ?
O59 Ni8 O55 91.4(4) . . ?
O37 Ni8 O55 88.6(3) 15_556 . ?
O49 Ni8 O55 107.8(3) . . ?
O59 Ni8 Ni8 52.2(2) . 10_556 ?
O37 Ni8 Ni8 55.92(9) 15_556 10_556 ?
O49 Ni8 Ni8 146.2(2) . 10_556 ?
O55 Ni8 Ni8 60.94(13) . 10_556 ?
O59 Ni8 O50 87.1(5) . 11_556 ?
O37 Ni8 O50 170.2(4) 15_556 11_556 ?
O49 Ni8 O50 86.5(4) . 11_556 ?
O55 Ni8 O50 81.9(4) . 11_556 ?
Ni8 Ni8 O50 120.1(4) 10_556 11_556 ?
O59 Ni8 O48 87.7(4) . . ?
O37 Ni8 O48 76.61(17) 15_556 . ?
O49 Ni8 O48 76.2(3) . . ?
O55 Ni8 O48 165.0(2) . . ?
Ni8 Ni8 O48 107.50(11) 10_556 . ?
O50 Ni8 O48 112.9(4) 11_556 . ?
O59 Ni8 Na6 122.5(8) . 8 ?
O37 Ni8 Na6 99.2(7) 15_556 8 ?
O49 Ni8 Na6 74.3(7) . 8 ?
O55 Ni8 Na6 34.5(7) . 8 ?
Ni8 Ni8 Na6 93.7(7) 10_556 8 ?
O50 Ni8 Na6 71.6(8) 11_556 8 ?
O48 Ni8 Na6 149.8(7) . 8 ?
O37 P1 O25 111.3(2) . . ?
O37 P1 O6 109.37(15) . 10 ?
O25 P1 O6 108.37(14) . 10 ?
O37 P1 O6 109.37(15) . . ?
O25 P1 O6 108.37(14) . . ?
O6 P1 O6 110.0(2) 10 . ?
O18 P2 O18 106.7(2) . 10 ?
O18 P2 O30 110.17(14) . 13 ?
O18 P2 O30 110.17(14) 10 13 ?
O18 P2 O8 109.84(14) . . ?
O18 P2 O8 109.84(14) 10 . ?
O30 P2 O8 110.0(2) 13 . ?
O29 P3 O7 110.12(14) . 13 ?
O29 P3 O7 110.12(14) . 6 ?
O7 P3 O7 111.4(2) 13 6 ?
O29 P3 O35 112.6(2) . . ?
O7 P3 O35 106.21(14) 13 . ?
O7 P3 O35 106.21(14) 6 . ?
O5 P4 O5 106.7(2) 10 . ?
O5 P4 O51 109.90(15) 10 . ?
O5 P4 O51 109.90(15) . . ?
O5 P4 O20 109.06(15) 10 . ?
O5 P4 O20 109.06(15) . . ?
O51 P4 O20 112.1(2) . . ?
O3 P5 O21 111.27(16) 6 6 ?
O3 P5 O17 106.97(17) 6 . ?
O21 P5 O17 112.56(17) 6 . ?
O3 P5 O39 109.07(18) 6 . ?
O21 P5 O39 108.41(18) 6 . ?
O17 P5 O39 108.48(19) . . ?
O23 P6 O40 111.7(3) . . ?
O23 P6 O15 109.23(15) . 10 ?
O40 P6 O15 108.33(16) . 10 ?
O23 P6 O15 109.23(15) . . ?
O40 P6 O15 108.33(16) . . ?
O15 P6 O15 110.0(2) 10 . ?
O28 P7 O4 112.85(17) . . ?
O28 P7 O11 112.93(17) . . ?
O4 P7 O11 104.07(17) . . ?
O28 P7 O41 108.98(17) . . ?
O4 P7 O41 107.77(18) . . ?
O11 P7 O41 110.06(18) . . ?
O28 P7 Na1 130.3(2) . . ?
O4 P7 Na1 48.5(2) . . ?
O11 P7 Na1 55.6(2) . . ?
O41 P7 Na1 120.5(2) . . ?
O42 P8 O26 115.36(15) . . ?
O42 P8 O26 115.36(15) . 10 ?
O26 P8 O26 105.3(2) . 10 ?
O42 P8 O43 104.9(2) . . ?
O26 P8 O43 107.79(15) . . ?
O26 P8 O43 107.79(15) 10 . ?
O44 P9 O14 108.92(16) . . ?
O44 P9 O14 108.92(16) . 10 ?
O14 P9 O14 108.5(3) . 10 ?
O44 P9 O38 110.6(3) . . ?
O14 P9 O38 109.93(16) . . ?
O14 P9 O38 109.93(16) 10 . ?
O16 P10 O45 109.7(2) . . ?
O16 P10 O31 113.00(19) . . ?
O45 P10 O31 112.6(2) . . ?
O16 P10 O46 108.1(2) . . ?
O45 P10 O46 107.6(2) . . ?
O31 P10 O46 105.42(19) . . ?
Mo4 O1 Mo1 82.93(11) . . ?
Mo4 O1 Ni1 132.24(15) . . ?
Mo1 O1 Ni1 135.54(15) . . ?
Mo4 O2 Mo1 83.50(11) . . ?
Mo4 O2 Ni4 134.54(15) . . ?
Mo1 O2 Ni4 138.07(15) . . ?
P5 O3 Mo1 139.13(19) 6 . ?
P5 O3 Na1 122.7(2) 6 . ?
Mo1 O3 Na1 96.85(19) . . ?
P7 O4 Mo1 144.17(19) . . ?
P7 O4 Na1 102.3(3) . . ?
Mo1 O4 Na1 111.7(3) . . ?
P4 O5 Mo1 122.37(16) . . ?
P1 O6 Mo2 137.72(18) . . ?
P3 O7 Mo2 136.01(17) 13 . ?
P2 O8 Mo2 114.80(9) . 10 ?
P2 O8 Mo2 114.80(9) . . ?
Mo2 O8 Mo2 129.34(16) 10 . ?
Mo2 O10 Mo3 82.46(10) . . ?
Mo2 O10 Ni3 130.90(14) . 6 ?
Mo3 O10 Ni3 136.23(14) . 6 ?
P7 O11 Mo3 139.02(19) . . ?
P7 O11 Na1 94.1(3) . . ?
Mo3 O11 Na1 126.6(3) . . ?
Mo2 O12 Mo3 83.31(10) . . ?
Mo2 O12 Ni2 132.05(14) . . ?
Mo3 O12 Ni2 141.73(14) . . ?
P9 O14 Mo4 138.6(2) . . ?
P6 O15 Mo4 135.79(19) . . ?
P10 O16 Ni1 123.6(2) . . ?
P5 O17 Mo3 138.30(18) . . ?
P2 O18 Mo3 123.59(16) . . ?
P4 O20 Mo4 114.77(9) . 10 ?
P4 O20 Mo4 114.77(9) . . ?
Mo4 O20 Mo4 128.68(18) 10 . ?
P5 O21 Ni3 133.37(17) 6 . ?
P5 O21 Ni1 133.80(16) 6 . ?
Ni3 O21 Ni1 92.77(11) . . ?
Ni2 O22 Ni2 100.31(17) 10 . ?
P6 O23 Ni1 131.07(14) . 10 ?
P6 O23 Ni1 131.07(14) . . ?
Ni1 O23 Ni1 84.97(16) 10 . ?
Ni1 O24 Ni1 81.88(13) 10 . ?
Ni1 O24 Ni3 87.67(6) 10 10 ?
Ni1 O24 Ni3 145.1(2) . 10 ?
Ni1 O24 Ni3 145.1(2) 10 . ?
Ni1 O24 Ni3 87.67(6) . . ?
Ni3 O24 Ni3 82.17(13) 10 . ?
P1 O25 Ni2 126.41(11) . . ?
P1 O25 Ni2 126.41(11) . 10 ?
Ni2 O25 Ni2 100.26(17) . 10 ?
P8 O26 Ni2 121.57(17) . . ?
P8 O26 Ni4 121.78(17) . . ?
Ni2 O26 Ni4 99.04(12) . . ?
P7 O28 Ni2 130.79(18) . . ?
P7 O28 Ni4 130.78(18) . . ?
Ni2 O28 Ni4 98.09(12) . . ?
P3 O29 Ni3 129.92(13) . 10 ?
P3 O29 Ni3 129.92(13) . . ?
Ni3 O29 Ni3 84.94(14) 10 . ?
P2 O30 Ni3 120.84(16) 13 10 ?
P2 O30 Ni3 120.84(16) 13 . ?
Ni3 O30 Ni3 88.16(16) 10 . ?
P10 O31 Ni3 125.26(18) . . ?
Ni4 O32 Ni4 105.81(19) 10 . ?
Ni5 O34 Na2 98.7(4) . 6 ?
P3 O35 Ni5 127.42(10) . 9_655 ?
P3 O35 Ni5 127.42(10) . . ?
Ni5 O35 Ni5 101.18(17) 9_655 . ?
Ni5 O36 Na2 100.7(3) . 6 ?
P1 O37 Ni8 144.99(11) . 15_455 ?
P1 O37 Ni8 144.99(11) . 8_455 ?
Ni8 O37 Ni8 68.15(18) 15_455 8_455 ?
P9 O38 Ni4 125.70(15) . 10 ?
P9 O38 Ni4 125.70(15) . . ?
Ni4 O38 Ni4 94.80(18) 10 . ?
P5 O39 Na8 120.5(6) . 16_556 ?
P6 O40 Ni6 144.06(10) . . ?
P6 O40 Ni6 144.06(10) . 10 ?
Ni6 O40 Ni6 70.37(16) . 10 ?
P9 O44 Ni6 143.50(12) . 2 ?
P9 O44 Ni6 143.50(12) . 9 ?
Ni6 O44 Ni6 69.24(17) 2 9 ?
P10 O46 Na2 141.8(4) . 5_545 ?
P10 O46 Na7 129.1(6) . 10 ?
Na2 O46 Na7 81.4(7) 5_545 10 ?
O47 O47 Ni7 73.5(2) 10 . ?
O47 O47 Na1 162.3(2) 10 . ?
Ni7 O47 Na1 90.4(3) . . ?
Ni8 O48 Na5 119.2(6) . . ?
Ni8 O48 Na5 94.1(5) . 6 ?
Na5 O48 Na5 26.2(10) . 6 ?
O9W O50 Ni8 102.4(11) . 11 ?
O9W O50 Na8 71.8(11) . . ?
Ni8 O50 Na8 129.4(8) 11 . ?
P4 O51 Ni1 119.24(16) . 10 ?
P4 O51 Ni1 119.24(16) . . ?
Ni1 O51 Ni1 87.91(16) 10 . ?
Mo1 O52 Na8 124.5(6) . 11_556 ?
Ni6 O53 Ni6 64.34(18) . 10 ?
Ni6 O53 Na6 108.9(10) . 14_545 ?
Ni6 O53 Na6 155.6(10) 10 14_545 ?
Ni6 O53 Na6 155.6(10) . 5_545 ?
Ni6 O53 Na6 108.9(10) 10 5_545 ?
Na6 O53 Na6 67(2) 14_545 5_545 ?
Ni6 O53 Na7 141.4(6) . 10 ?
Ni6 O53 Na7 81.0(6) 10 10 ?
Na6 O53 Na7 95.5(12) 14_545 10 ?
Na6 O53 Na7 29.0(11) 5_545 10 ?
Ni6 O53 Na7 81.0(6) . . ?
Ni6 O53 Na7 141.4(6) 10 . ?
Na6 O53 Na7 29.0(11) 14_545 . ?
Na6 O53 Na7 95.5(12) 5_545 . ?
Na7 O53 Na7 123.5(11) 10 . ?
Ni6 O54 Na4 116.0(9) . . ?
Ni8 O55 Ni8 58.1(3) 10_556 . ?
Ni8 O55 Na6 156.0(13) 10_556 8 ?
Ni8 O55 Na6 106.5(12) . 8 ?
Ni8 O55 Na6 106.5(12) 10_556 15_556 ?
Ni8 O55 Na6 156.0(13) . 15_556 ?
Na6 O55 Na6 81(2) 8 15_556 ?
O58 O56 Ni6 88.6(6) . . ?
O58 O56 Na7 70.1(9) . . ?
Ni6 O56 Na7 98.4(8) . . ?
Na8 O57 Ni6 120.6(8) . . ?
O56 O58 Na3 173.9(8) . . ?
O56 O58 Na7 74.1(9) . . ?
Na3 O58 Na7 101.8(9) . . ?
O56 O58 Na6 106.5(12) . 14_545 ?
Na3 O58 Na6 70.7(10) . 14_545 ?
Na7 O58 Na6 34.8(12) . 14_545 ?
Ni8 O59 Ni8 75.6(5) . 10_556 ?
Ni7 O60 Na1 101.0(4) . . ?
Ni7 O60 Na1 86.7(3) . 6 ?
Na1 O60 Na1 53.4(4) . 6 ?
Na2 O4W Na2 143.1(7) 8 5_545 ?
Na1 O5W O5W 115.5(7) . 6 ?
Na1 O5W Na1 88.1(9) . 6 ?
O5W O5W Na1 29.0(4) 6 6 ?
Na1 O5W Na5 153.2(10) . 6 ?
O5W O5W Na5 89.3(6) 6 6 ?
Na1 O5W Na5 117.8(7) 6 6 ?
Na1 O5W Na5 170.2(11) . . ?
O5W O5W Na5 61.4(5) 6 . ?
Na1 O5W Na5 90.0(6) 6 . ?
Na5 O5W Na5 27.9(9) 6 . ?
O8W O7W Na2 131.3(16) 6 6 ?
O8W O7W Na6 67.6(15) 6 6 ?
Na2 O7W Na6 115.2(13) 6 6 ?
O8W O7W Na7 95.4(14) 6 9_655 ?
Na2 O7W Na7 93.4(9) 6 9_655 ?
Na6 O7W Na7 28.3(11) 6 9_655 ?
O7W O8W Na6 84.4(17) 6 . ?
O7W O8W Na2 29.5(11) 6 . ?
Na6 O8W Na2 92.2(13) . . ?
O50 O9W Na8 76.0(12) . . ?
O50 O9W Na7 107.9(13) . . ?
Na8 O9W Na7 55.6(9) . . ?
O50 O9W Na6 112.0(14) . 14_545 ?
Na8 O9W Na6 84.7(12) . 14_545 ?
Na7 O9W Na6 30.3(11) . 14_545 ?
O5W Na1 O5W 35.4(6) . 6 ?
O5W Na1 O4 110.3(7) . . ?
O5W Na1 O4 143.8(5) 6 . ?
O5W Na1 O60 127.4(7) . . ?
O5W Na1 O60 94.9(5) 6 . ?
O4 Na1 O60 109.5(4) . . ?
O5W Na1 Na1 63.2(7) . 6 ?
O5W Na1 Na1 28.7(4) 6 6 ?
O4 Na1 Na1 171.7(4) . 6 ?
O60 Na1 Na1 73.3(3) . 6 ?
O5W Na1 O11 96.7(7) . . ?
O5W Na1 O11 120.5(5) 6 . ?
O4 Na1 O11 59.4(2) . . ?
O60 Na1 O11 133.3(4) . . ?
Na1 Na1 O11 124.7(7) 6 . ?
O5W Na1 O3 99.4(8) . . ?
O5W Na1 O3 102.5(5) 6 . ?
O4 Na1 O3 64.5(3) . . ?
O60 Na1 O3 69.0(3) . . ?
Na1 Na1 O3 110.6(5) 6 . ?
O11 Na1 O3 123.8(3) . . ?
O5W Na1 O47 157.9(9) . . ?
O5W Na1 O47 131.4(5) 6 . ?
O4 Na1 O47 84.8(3) . . ?
O60 Na1 O47 56.6(3) . . ?
Na1 Na1 O47 102.9(3) 6 . ?
O11 Na1 O47 76.8(3) . . ?
O3 Na1 O47 101.7(3) . . ?
O5W Na1 O60 104.9(8) . 6 ?
O5W Na1 O60 78.9(4) 6 6 ?
O4 Na1 O60 134.9(4) . 6 ?
O60 Na1 O60 66.8(4) . 6 ?
Na1 Na1 O60 53.4(3) 6 6 ?
O11 Na1 O60 89.7(3) . 6 ?
O3 Na1 O60 135.6(4) . 6 ?
O47 Na1 O60 54.6(3) . 6 ?
O5W Na1 P7 105.1(7) . . ?
O5W Na1 P7 138.9(5) 6 . ?
O4 Na1 P7 29.24(12) . . ?
O60 Na1 P7 126.1(4) . . ?
Na1 Na1 P7 154.2(6) 6 . ?
O11 Na1 P7 30.22(11) . . ?
O3 Na1 P7 93.6(3) . . ?
O47 Na1 P7 80.0(2) . . ?
O60 Na1 P7 114.5(3) 6 . ?
O5W Na1 Ni7 132.0(8) . . ?
O5W Na1 Ni7 97.7(4) 6 . ?
O4 Na1 Ni7 117.7(3) . . ?
O60 Na1 Ni7 34.8(2) . . ?
Na1 Na1 Ni7 69.19(14) 6 . ?
O11 Na1 Ni7 105.6(3) . . ?
O3 Na1 Ni7 102.2(3) . . ?
O47 Na1 Ni7 35.81(17) . . ?
O60 Na1 Ni7 35.47(17) 6 . ?
P7 Na1 Ni7 115.6(3) . . ?
O5W Na1 Mo1 115.9(8) . . ?
O5W Na1 Mo1 134.0(5) 6 . ?
O4 Na1 Mo1 31.68(16) . . ?
O60 Na1 Mo1 83.9(3) . . ?
Na1 Na1 Mo1 144.7(6) 6 . ?
O11 Na1 Mo1 90.5(2) . . ?
O3 Na1 Mo1 34.61(13) . . ?
O47 Na1 Mo1 85.5(3) . . ?
O60 Na1 Mo1 138.9(3) 6 . ?
P7 Na1 Mo1 60.58(16) . . ?
Ni7 Na1 Mo1 106.0(2) . . ?
O7W Na2 O2W 108.6(10) 6 . ?
O7W Na2 O46 107.1(9) 6 5_455 ?
O2W Na2 O46 116.3(7) . 5_455 ?
O7W Na2 O36 88.3(8) 6 6 ?
O2W Na2 O36 153.7(7) . 6 ?
O46 Na2 O36 75.5(5) 5_455 6 ?
O7W Na2 O34 106.7(8) 6 6 ?
O2W Na2 O34 85.5(5) . 6 ?
O46 Na2 O34 130.2(7) 5_455 6 ?
O36 Na2 O34 70.1(4) 6 6 ?
O7W Na2 O8W 19.2(7) 6 . ?
O2W Na2 O8W 126.5(9) . . ?
O46 Na2 O8W 100.9(7) 5_455 . ?
O36 Na2 O8W 69.1(6) 6 . ?
O34 Na2 O8W 99.2(6) 6 . ?
O7W Na2 O4W 175.3(10) 6 5_455 ?
O2W Na2 O4W 72.8(5) . 5_455 ?
O46 Na2 O4W 75.7(5) 5_455 5_455 ?
O36 Na2 O4W 88.8(5) 6 5_455 ?
O34 Na2 O4W 68.9(5) 6 5_455 ?
O8W Na2 O4W 157.6(8) . 5_455 ?
O7W Na2 Na6 38.7(9) 6 . ?
O2W Na2 Na6 122.0(9) . . ?
O46 Na2 Na6 68.8(8) 5_455 . ?
O36 Na2 Na6 83.8(8) 6 . ?
O34 Na2 Na6 138.3(9) 6 . ?
O8W Na2 Na6 39.9(8) . . ?
O4W Na2 Na6 144.4(9) 5_455 . ?
O7W Na2 Na7 57.7(8) 6 14_455 ?
O2W Na2 Na7 107.8(7) . 14_455 ?
O46 Na2 Na7 55.5(5) 5_455 14_455 ?
O36 Na2 Na7 98.2(6) 6 14_455 ?
O34 Na2 Na7 161.7(7) 6 14_455 ?
O8W Na2 Na7 62.9(7) . 14_455 ?
O4W Na2 Na7 126.4(7) 5_455 14_455 ?
Na6 Na2 Na7 23.4(8) . 14_455 ?
O7W Na2 Ni5 99.8(8) 6 5_455 ?
O2W Na2 Ni5 119.9(5) . 5_455 ?
O46 Na2 Ni5 103.4(6) 5_455 5_455 ?
O36 Na2 Ni5 35.0(2) 6 5_455 ?
O34 Na2 Ni5 35.2(2) 6 5_455 ?
O8W Na2 Ni5 83.7(6) . 5_455 ?
O4W Na2 Ni5 75.8(4) 5_455 5_455 ?
Na6 Na2 Ni5 113.4(8) . 5_455 ?
Na7 Na2 Ni5 132.0(6) 14_455 5_455 ?
O58 Na3 O58 84.7(6) . 10 ?
O58 Na3 Na6 59.3(9) . 14_545 ?
O58 Na3 Na6 98.6(10) 10 14_545 ?
O58 Na3 Na6 98.6(10) . 5_545 ?
O58 Na3 Na6 59.3(9) 10 5_545 ?
Na6 Na3 Na6 58.7(18) 14_545 5_545 ?
O58 Na3 Na7 39.5(6) . . ?
O58 Na3 Na7 103.6(6) 10 . ?
Na6 Na3 Na7 23.0(10) 14_545 . ?
Na6 Na3 Na7 79.2(10) 5_545 . ?
O58 Na3 Na7 103.6(6) . 10 ?
O58 Na3 Na7 39.5(6) 10 10 ?
Na6 Na3 Na7 79.2(10) 14_545 10 ?
Na6 Na3 Na7 23.0(10) 5_545 10 ?
Na7 Na3 Na7 96.8(9) . 10 ?
Na4 Na4 O54 127.8(8) 9 2 ?
Na4 Na4 O54 127.8(8) 9 . ?
O54 Na4 O54 104.5(17) 2 . ?
Na5 Na5 O6W 153(2) 6 16_556 ?
Na5 Na5 O48 106.6(17) 6 . ?
O6W Na5 O48 97.4(9) 16_556 . ?
Na5 Na5 O5W 90.7(6) 6 6 ?
O6W Na5 O5W 81.7(7) 16_556 6 ?
O48 Na5 O5W 131.9(10) . 6 ?
Na5 Na5 O48 47.2(12) 6 6 ?
O6W Na5 O48 116.8(9) 16_556 6 ?
O48 Na5 O48 101.7(7) . 6 ?
O5W Na5 O48 121.7(8) 6 6 ?
Na5 Na5 O5W 61.4(5) 6 . ?
O6W Na5 O5W 108.0(8) 16_556 . ?
O48 Na5 O5W 136.8(10) . . ?
O5W Na5 O5W 29.3(5) 6 . ?
O48 Na5 O5W 97.2(7) 6 . ?
Na5 Na5 Na1 98.6(4) 6 6 ?
O6W Na5 Na1 73.2(6) 16_556 6 ?
O48 Na5 Na1 131.1(8) . 6 ?
O5W Na5 Na1 8.5(3) 6 6 ?
O48 Na5 Na1 125.7(6) 6 6 ?
O5W Na5 Na1 37.3(3) . 6 ?
Na5 Na5 Na1 62.2(4) 6 . ?
O6W Na5 Na1 108.5(7) 16_556 . ?
O48 Na5 Na1 134.1(9) . . ?
O5W Na5 Na1 28.7(4) 6 . ?
O48 Na5 Na1 99.3(5) 6 . ?
O5W Na5 Na1 2.8(3) . . ?
Na1 Na5 Na1 36.9(3) 6 . ?
Na7 Na6 O8W 126(3) 14_455 . ?
Na7 Na6 O55 127(3) 14_455 15_455 ?
O8W Na6 O55 93.0(17) . 15_455 ?
Na7 Na6 O7W 98(2) 14_455 6 ?
O8W Na6 O7W 28.0(8) . 6 ?
O55 Na6 O7W 109.2(18) 15_455 6 ?
Na7 Na6 O58 63.6(19) 14_455 14_455 ?
O8W Na6 O58 128.2(19) . 14_455 ?
O55 Na6 O58 122.6(19) 15_455 14_455 ?
O7W Na6 O58 125.9(18) 6 14_455 ?
Na7 Na6 O53 96(2) 14_455 5_455 ?
O8W Na6 O53 138(2) . 5_455 ?
O55 Na6 O53 58.8(11) 15_455 5_455 ?
O7W Na6 O53 165(2) 6 5_455 ?
O58 Na6 O53 64.2(11) 14_455 5_455 ?
Na7 Na6 Na3 109(2) 14_455 5_455 ?
O8W Na6 Na3 85.1(14) . 5_455 ?
O55 Na6 Na3 109.7(17) 15_455 5_455 ?
O7W Na6 Na3 100.5(15) 6 5_455 ?
O58 Na6 Na3 50.0(8) 14_455 5_455 ?
O53 Na6 Na3 78.0(12) 5_455 5_455 ?
Na7 Na6 Na6 151(2) 14_455 10 ?
O8W Na6 Na6 82.0(12) . 10 ?
O55 Na6 Na6 49.6(12) 15_455 10 ?
O7W Na6 Na6 109.9(11) 6 10 ?
O58 Na6 Na6 93.6(10) 14_455 10 ?
O53 Na6 Na6 56.6(10) 5_455 10 ?
Na3 Na6 Na6 60.7(9) 5_455 10 ?
Na7 Na6 O9W 70(2) 14_455 14_455 ?
O8W Na6 O9W 137.8(19) . 14_455 ?
O55 Na6 O9W 57.2(11) 15_455 14_455 ?
O7W Na6 O9W 129.1(17) 6 14_455 ?
O58 Na6 O9W 93.9(14) 14_455 14_455 ?
O53 Na6 O9W 53.7(9) 5_455 14_455 ?
Na3 Na6 O9W 130.4(16) 5_455 14_455 ?
Na6 Na6 O9W 95.8(9) 10 14_455 ?
Na7 Na6 Na2 79(2) 14_455 . ?
O8W Na6 Na2 47.9(9) . . ?
O55 Na6 Na2 135.2(17) 15_455 . ?
O7W Na6 Na2 26.1(7) 6 . ?
O58 Na6 Na2 101.2(13) 14_455 . ?
O53 Na6 Na2 165.0(17) 5_455 . ?
Na3 Na6 Na2 90.3(11) 5_455 . ?
Na6 Na6 Na2 125.3(7) 10 . ?
O9W Na6 Na2 134.5(15) 14_455 . ?
Na7 Na6 Na8 30.6(16) 14_455 14_455 ?
O8W Na6 Na8 132.3(17) . 14_455 ?
O55 Na6 Na8 96.9(15) 15_455 14_455 ?
O7W Na6 Na8 106.2(15) 6 14_455 ?
O58 Na6 Na8 83.3(12) 14_455 14_455 ?
O53 Na6 Na8 84.5(12) 5_455 14_455 ?
Na3 Na6 Na8 133.3(15) 5_455 14_455 ?
Na6 Na6 Na8 137.0(8) 10 14_455 ?
O9W Na6 Na8 42.1(8) 14_455 14_455 ?
Na2 Na6 Na8 97.1(11) . 14_455 ?
Na7 Na6 Ni8 103(2) 14_455 8_455 ?
O8W Na6 Ni8 85.8(13) . 8_455 ?
O55 Na6 Ni8 39.0(8) 15_455 8_455 ?
O7W Na6 Ni8 85.7(12) 6 8_455 ?
O58 Na6 Ni8 145.7(16) 14_455 8_455 ?
O53 Na6 Ni8 88.0(12) 5_455 8_455 ?
Na3 Na6 Ni8 146.7(15) 5_455 8_455 ?
Na6 Na6 Ni8 86.3(7) 10 8_455 ?
O9W Na6 Ni8 52.1(8) 14_455 8_455 ?
Na2 Na6 Ni8 106.8(11) . 8_455 ?
Na8 Na6 Ni8 73.9(9) 14_455 8_455 ?
Na6 Na7 O58 82(2) 14_545 . ?
Na6 Na7 O56 115(2) 14_545 . ?
O58 Na7 O56 35.8(6) . . ?
Na6 Na7 Na8 131(2) 14_545 . ?
O58 Na7 Na8 122.0(14) . . ?
O56 Na7 Na8 88.7(12) . . ?
Na6 Na7 O9W 80(2) 14_545 . ?
O58 Na7 O9W 103.1(11) . . ?
O56 Na7 O9W 95.4(11) . . ?
Na8 Na7 O9W 55.1(9) . . ?
Na6 Na7 O46 100(2) 14_545 10 ?
O58 Na7 O46 73.1(8) . 10 ?
O56 Na7 O46 81.6(8) . 10 ?
Na8 Na7 O46 126.8(12) . 10 ?
O9W Na7 O46 176.2(12) . 10 ?
Na6 Na7 O53 55.1(19) 14_545 . ?
O58 Na7 O53 58.5(7) . . ?
O56 Na7 O53 72.5(8) . . ?
Na8 Na7 O53 98.8(11) . . ?
O9W Na7 O53 49.9(6) . . ?
O46 Na7 O53 126.7(10) 10 . ?
Na6 Na7 O7W 53.5(19) 14_545 9_655 ?
O58 Na7 O7W 112.5(11) . 9_655 ?
O56 Na7 O7W 143.9(12) . 9_655 ?
Na8 Na7 O7W 125.5(13) . 9_655 ?
O9W Na7 O7W 112.8(11) . 9_655 ?
O46 Na7 O7W 69.1(7) 10 9_655 ?
O53 Na7 O7W 108.5(9) . 9_655 ?
Na6 Na7 Ni6 93(2) 14_545 . ?
O58 Na7 Ni6 48.7(6) . . ?
O56 Na7 Ni6 38.9(5) . . ?
Na8 Na7 Ni6 79.2(10) . . ?
O9W Na7 Ni6 59.0(7) . . ?
O46 Na7 Ni6 117.5(9) 10 . ?
O53 Na7 Ni6 39.1(4) . . ?
O7W Na7 Ni6 146.1(10) 9_655 . ?
Na6 Na7 Na3 48.1(19) 14_545 . ?
O58 Na7 Na3 38.7(6) . . ?
O56 Na7 Na3 74.5(8) . . ?
Na8 Na7 Na3 156.1(13) . . ?
O9W Na7 Na3 108.8(10) . . ?
O46 Na7 Na3 68.3(6) 10 . ?
O53 Na7 Na3 60.3(5) . . ?
O7W Na7 Na3 75.5(7) 9_655 . ?
Ni6 Na7 Na3 77.0(6) . . ?
Na6 Na7 Na2 78(2) 14_545 14_545 ?
O58 Na7 Na2 106.1(10) . 14_545 ?
O56 Na7 Na2 124.4(11) . 14_545 ?
Na8 Na7 Na2 124.6(12) . 14_545 ?
O9W Na7 Na2 139.6(11) . 14_545 ?
O46 Na7 Na2 43.0(5) 10 14_545 ?
O53 Na7 Na2 131.0(10) . 14_545 ?
O7W Na7 Na2 28.9(5) 9_655 14_545 ?
Ni6 Na7 Na2 154.5(9) . 14_545 ?
Na3 Na7 Na2 79.3(7) . 14_545 ?
Na6 Na7 Na6 18.9(15) 14_545 5_545 ?
O58 Na7 Na6 67.7(9) . 5_545 ?
O56 Na7 Na6 97.8(11) . 5_545 ?
Na8 Na7 Na6 127.1(13) . 5_545 ?
O9W Na7 Na6 72.0(9) . 5_545 ?
O46 Na7 Na6 106.0(10) 10 5_545 ?
O53 Na7 Na6 37.2(7) . 5_545 ?
O7W Na7 Na6 72.0(9) 9_655 5_545 ?
Ni6 Na7 Na6 74.4(8) . 5_545 ?
Na3 Na7 Na6 42.2(7) . 5_545 ?
Na2 Na7 Na6 94.1(9) 14_545 5_545 ?
O57 Na8 O9W 50.6(7) . . ?
O57 Na8 Na7 90.2(12) . . ?
O9W Na8 Na7 69.3(11) . . ?
O57 Na8 O50 73.6(8) . . ?
O9W Na8 O50 32.3(6) . . ?
Na7 Na8 O50 88.7(11) . . ?
O57 Na8 O3W 95.1(9) . 11 ?
O9W Na8 O3W 135.7(12) . 11 ?
Na7 Na8 O3W 86.4(10) . 11 ?
O50 Na8 O3W 167.7(12) . 11 ?
O57 Na8 O39 172.7(13) . 16_545 ?
O9W Na8 O39 122.2(11) . 16_545 ?
Na7 Na8 O39 87.7(11) . 16_545 ?
O50 Na8 O39 99.4(9) . 16_545 ?
O3W Na8 O39 91.7(8) 11 16_545 ?
O57 Na8 O52 85.9(9) . 11 ?
O9W Na8 O52 119.4(11) . 11 ?
Na7 Na8 O52 163.0(13) . 11 ?
O50 Na8 O52 106.0(9) . 11 ?
O3W Na8 O52 77.5(7) 11 11 ?
O39 Na8 O52 98.1(8) 16_545 11 ?
O57 Na8 Na6 84.7(10) . 14_545 ?
O9W Na8 Na6 53.2(9) . 14_545 ?
Na7 Na8 Na6 18.1(10) . 14_545 ?
O50 Na8 Na6 70.6(10) . 14_545 ?
O3W Na8 Na6 104.0(10) 11 14_545 ?
O39 Na8 Na6 91.2(10) 16_545 14_545 ?
O52 Na8 Na6 170.6(12) 11 14_545 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O52 1.678(3) . ?
Mo1 O2 1.957(3) . ?
Mo1 O1 1.980(3) . ?
Mo1 O4 2.059(3) . ?
Mo1 O3 2.083(3) . ?
Mo1 O5 2.191(3) . ?
Mo1 Mo4 2.5981(6) . ?
Mo1 Na1 3.642(10) . ?
Mo2 O9 1.677(3) . ?
Mo2 O12 1.936(3) . ?
Mo2 O10 1.950(3) . ?
Mo2 O6 2.047(3) . ?
Mo2 O7 2.060(3) . ?
Mo2 O8 2.4146(17) . ?
Mo2 Mo3 2.5919(6) . ?
Mo3 O19 1.685(3) . ?
Mo3 O12 1.963(3) . ?
Mo3 O10 1.982(3) . ?
Mo3 O11 2.071(3) . ?
Mo3 O17 2.092(3) . ?
Mo3 O18 2.198(3) . ?
Mo4 O13 1.697(3) . ?
Mo4 O1 1.943(3) . ?
Mo4 O2 1.945(3) . ?
Mo4 O15 2.034(3) . ?
Mo4 O14 2.037(3) . ?
Mo4 O20 2.3802(19) . ?
Ni1 O16 2.004(3) . ?
Ni1 O51 2.025(3) . ?
Ni1 O1 2.049(3) . ?
Ni1 O21 2.065(3) . ?
Ni1 O23 2.081(3) . ?
Ni1 O24 2.145(3) . ?
Ni1 Ni1 2.8111(12) 10 ?
Ni1 Ni3 2.9753(9) . ?
Ni2 O12 2.040(3) . ?
Ni2 O26 2.068(3) . ?
Ni2 O22 2.081(3) . ?
Ni2 O25 2.081(3) . ?
Ni2 O28 2.090(3) . ?
Ni2 O27 2.099(3) . ?
Ni3 O30 2.032(3) . ?
Ni3 O31 2.036(3) . ?
Ni3 O21 2.044(3) . ?
Ni3 O10 2.080(3) 6 ?
Ni3 O29 2.093(3) . ?
Ni3 O24 2.151(3) . ?
Ni3 Ni3 2.8269(11) 10 ?
Ni4 O32 2.043(3) . ?
Ni4 O33 2.057(4) . ?
Ni4 O2 2.067(3) . ?
Ni4 O26 2.112(3) . ?
Ni4 O28 2.121(3) . ?
Ni4 O38 2.214(3) . ?
Ni5 O35 2.036(2) . ?
Ni5 O35 2.036(2) 9_655 ?
Ni5 O34 2.067(4) . ?
Ni5 O34 2.067(4) 2_655 ?
Ni5 O36 2.069(3) . ?
Ni5 O36 2.069(3) 2_655 ?
Ni5 Na2 3.549(15) 6 ?
Ni5 Na2 3.549(15) 5_545 ?
Ni6 O40 1.953(4) . ?
Ni6 O44 1.981(4) 9 ?
Ni6 O54 2.069(7) . ?
Ni6 O53 2.113(5) . ?
Ni6 O56 2.099(9) . ?
Ni6 O57 2.142(10) . ?
Ni6 Ni6 2.251(3) 10 ?
Ni6 Na7 3.31(3) . ?
Ni7 O60 2.047(8) 13 ?
Ni7 O60 2.047(8) 6 ?
Ni7 O60 2.047(8) . ?
Ni7 O60 2.047(8) 10 ?
Ni7 O47 2.061(7) 6 ?
Ni7 O47 2.061(7) 13 ?
Ni7 O47 2.061(7) 10 ?
Ni7 O47 2.061(7) . ?
Ni7 Na1 3.522(9) 6 ?
Ni7 Na1 3.522(9) 10 ?
Ni7 Na1 3.522(9) 13 ?
Ni7 Na1 3.522(9) . ?
Ni8 O59 1.788(9) . ?
Ni8 O37 1.957(4) 15_556 ?
Ni8 O49 2.157(8) . ?
Ni8 O55 2.257(9) . ?
Ni8 Ni8 2.193(4) 10_556 ?
Ni8 O50 2.204(12) 11_556 ?
Ni8 O48 2.203(4) . ?
Ni8 Na6 3.44(4) 8 ?
P1 O37 1.502(4) . ?
P1 O25 1.548(4) . ?
P1 O6 1.544(3) 10 ?
P1 O6 1.544(3) . ?
P2 O18 1.531(3) . ?
P2 O18 1.531(3) 10 ?
P2 O30 1.543(4) 13 ?
P2 O8 1.556(4) . ?
P3 O29 1.521(4) . ?
P3 O7 1.532(3) 13 ?
P3 O7 1.532(3) 6 ?
P3 O35 1.539(4) . ?
P4 O5 1.546(3) 10 ?
P4 O5 1.546(3) . ?
P4 O51 1.557(4) . ?
P4 O20 1.591(4) . ?
P5 O3 1.527(3) 6 ?
P5 O21 1.528(3) 6 ?
P5 O17 1.537(3) . ?
P5 O39 1.565(3) . ?
P6 O23 1.517(4) . ?
P6 O40 1.528(4) . ?
P6 O15 1.550(3) 10 ?
P6 O15 1.550(3) . ?
P7 O28 1.524(3) . ?
P7 O4 1.525(3) . ?
P7 O11 1.540(3) . ?
P7 O41 1.555(3) . ?
P7 Na1 3.051(8) . ?
P8 O42 1.507(4) . ?
P8 O26 1.541(3) . ?
P8 O26 1.541(3) 10 ?
P8 O43 1.596(4) . ?
P9 O44 1.500(5) . ?
P9 O14 1.547(3) . ?
P9 O14 1.547(3) 10 ?
P9 O38 1.551(5) . ?
P10 O16 1.527(4) . ?
P10 O45 1.537(4) . ?
P10 O31 1.554(3) . ?
P10 O46 1.585(4) . ?
O3 P5 1.527(3) 6 ?
O3 Na1 2.748(11) . ?
O4 Na1 2.337(9) . ?
O7 P3 1.532(3) 13 ?
O8 Mo2 2.4146(17) 10 ?
O10 Ni3 2.080(3) 6 ?
O11 Na1 2.525(9) . ?
O20 Mo4 2.3802(19) 10 ?
O21 P5 1.528(3) 6 ?
O22 Ni2 2.081(3) 10 ?
O23 Ni1 2.081(3) 10 ?
O24 Ni1 2.145(3) 10 ?
O24 Ni3 2.151(3) 10 ?
O25 Ni2 2.081(3) 10 ?
O29 Ni3 2.093(3) 10 ?
O30 P2 1.543(4) 13 ?
O30 Ni3 2.032(3) 10 ?
O32 Ni4 2.043(3) 10 ?
O34 Na2 2.588(14) 6 ?
O35 Ni5 2.036(2) 9_655 ?
O36 Na2 2.525(16) 6 ?
O37 Ni8 1.957(4) 15_455 ?
O37 Ni8 1.957(4) 8_455 ?
O38 Ni4 2.214(3) 10 ?
O39 Na8 2.52(2) 16_556 ?
O40 Ni6 1.953(4) 10 ?
O44 Ni6 1.981(4) 2 ?
O44 Ni6 1.981(4) 9 ?
O46 Na2 2.405(15) 5_545 ?
O46 Na7 2.90(3) 10 ?
O47 O47 1.170(15) 10 ?
O47 Na1 2.842(11) . ?
O48 Na5 2.28(2) . ?
O48 Na5 2.97(2) 6 ?
O50 O9W 1.29(2) . ?
O50 Ni8 2.204(12) 11 ?
O50 Na8 2.35(3) . ?
O51 Ni1 2.025(3) 10 ?
O52 Na8 2.55(2) 11_556 ?
O53 Ni6 2.113(5) 10 ?
O53 Na6 2.39(4) 14_545 ?
O53 Na6 2.39(4) 5_545 ?
O53 Na7 2.90(3) 10 ?
O53 Na7 2.90(3) . ?
O54 Na4 2.51(3) . ?
O55 Ni8 2.257(9) 10_556 ?
O55 Na6 2.03(4) 8 ?
O55 Na6 2.03(4) 15_556 ?
O56 O58 1.380(14) . ?
O56 Na7 2.27(3) . ?
O57 Na8 2.08(3) . ?
O58 Na3 2.180(13) . ?
O58 Na7 2.22(3) . ?
O58 Na6 2.45(4) 14_545 ?
O59 Ni8 1.788(9) 10_556 ?
O60 Na1 2.502(12) . ?
O60 Na1 2.987(12) 6 ?
O2W Na2 2.167(17) . ?
O3W Na8 2.52(3) 11_556 ?
O4W Na2 2.698(17) 8 ?
O4W Na2 2.698(17) 5_545 ?
O5W Na1 1.202(15) . ?
O5W O5W 1.44(2) 6 ?
O5W Na1 2.234(14) 6 ?
O5W Na5 2.57(2) 6 ?
O5W Na5 2.93(2) . ?
O6W Na5 2.30(3) 16_545 ?
O7W O8W 1.13(2) 6 ?
O7W Na2 1.69(2) 6 ?
O7W Na6 2.40(4) 6 ?
O7W Na7 2.95(3) 9_655 ?
O8W O7W 1.13(2) 6 ?
O8W Na6 2.23(4) . ?
O8W Na2 2.58(2) . ?
O9W Na8 2.30(3) . ?
O9W Na7 2.63(3) . ?
O9W Na6 2.75(4) 14_545 ?
O10W O10W 0.82(5) 4_554 ?
Na1 O5W 2.234(14) 6 ?
Na1 Na1 2.502(17) 6 ?
Na1 O60 2.987(12) 6 ?
Na2 O7W 1.69(2) 6 ?
Na2 O46 2.405(15) 5_455 ?
Na2 O36 2.525(16) 6 ?
Na2 O34 2.588(14) 6 ?
Na2 O4W 2.698(17) 5_455 ?
Na2 Na6 3.47(4) . ?
Na2 Na7 3.48(3) 14_455 ?
Na2 Ni5 3.549(15) 5_455 ?
Na3 O58 2.180(13) 10 ?
Na3 Na6 2.69(4) 14_545 ?
Na3 Na6 2.69(4) 5_545 ?
Na3 Na7 3.41(3) . ?
Na3 Na7 3.41(3) 10 ?
Na4 Na4 1.00(9) 9 ?
Na4 O54 2.51(3) 2 ?
Na5 Na5 1.37(5) 6 ?
Na5 O6W 2.30(3) 16_556 ?
Na5 O5W 2.57(2) 6 ?
Na5 O48 2.97(2) 6 ?
Na5 Na1 3.685(19) 6 ?
Na6 Na7 1.41(5) 14_455 ?
Na6 O55 2.03(4) 15_455 ?
Na6 O7W 2.40(4) 6 ?
Na6 O58 2.45(4) 14_455 ?
Na6 O53 2.39(4) 5_455 ?
Na6 Na3 2.69(4) 5_455 ?
Na6 Na6 2.63(8) 10 ?
Na6 O9W 2.75(4) 14_455 ?
Na6 Na8 3.42(5) 14_455 ?
Na6 Ni8 3.44(4) 8_455 ?
Na7 Na6 1.41(5) 14_545 ?
Na7 Na8 2.32(4) . ?
Na7 O46 2.90(3) 10 ?
Na7 O7W 2.95(3) 9_655 ?
Na7 Na2 3.48(3) 14_545 ?
Na7 Na6 3.93(5) 5_545 ?
Na8 O3W 2.52(3) 11 ?
Na8 O39 2.52(2) 16_545 ?
Na8 O52 2.55(2) 11 ?
Na8 Na6 3.42(5) 14_545 ?
